Lafarge cement plant in Contes,
From Wikipedia, the free encyclopedia
A cement is a binder, a substance that sets and hardens independently, and can bind
other materials together. The word "cement" traces to the Romans, who used the
term opus caementicium to describe masonry resembling modern concrete that was
made from crushed rock with burnt lime as binder. The volcanic ash and pulverized
brick additives that were added to the burnt lime to obtain a hydraulic binder were
later referred to as cementum, cimentum, cäment, and cement.
Cements used in construction can be characterized as being either hydraulic or non-
hydraulic. Hydraulic cements (e.g., Portland cement) harden because of hydration, a
chemical reaction between the anhydrous cement powder and water. Thus, they can
harden underwater or when constantly exposed to wet weather. The chemical
reaction results in hydrates that are not very water-soluble and so are quite durable in
water. Non-hydraulic cements do not harden underwater; for example, slaked limes
harden by reaction with atmospheric carbon dioxide.
The most important uses of cement are as an ingredient in the production of mortar in masonry, and of concrete, a combination
of cement and an aggregate to form a strong building material.
2 History of the origin of cement
2.1 Early uses
2.2 Modern cements
3 Types of modern cement
3.1 Portland cement
3.2 Energetically modified cement
3.3 Portland cement blends
3.4 Non-Portland hydraulic cements
4 Curing (Setting)
5 Safety issues
6 Cement industry in the world
7 Environmental impacts
7.1 CO2 emissions
7.2 Heavy metal emissions in the air
7.3 Heavy metals present in the clinker
7.4 Use of alternative fuels and by-products materials
8 Green cement
9 See also
11 Further reading
12 External links
Non-hydraulic cement such as slaked limes (calcium hydroxide mixed with water), harden due to the reaction of carbonation in
presence of the carbon dioxide naturally present in the air. Calcium oxide is produced by lime calcination at temperatures above
825 °C (1,517 °F) for about 10 hours at atmospheric pressure:
CaCO3 → CaO + CO2
The calcium oxide is then spent mixing it to water to make slaked lime:
CaO + H2O → Ca(OH)2
Once the water in excess from the slaked lime is completely evaporated (this process is technically called setting), the
Ca(OH)2 + CO2 → CaCO3 + H2O
This reaction takes a significant amount of time because the partial pressure of carbon dioxide in the air is small. The reaction of
carbonation requires the air be in contact with the dry cement, hence, for this reason the slaked lime is a non-hydraulic cement
and cannot be used under water.
Conversely, the chemistry ruling the action of the hydraulic cement is the hydration. Hydraulic cements (such as the Portland
cement) are made of a mixture of silicates and oxides, the four main components being:
The reactions during the setting of the cement are:
(3CaO·Al2O3)2 + (x+8) H2O → 4 CaO·Al2O3·xH2O + 2 CaO·Al2O3·8H2O
(3CaO·Al2O3) + 12 H2O + Ca(OH)2 → 4 CaO·Al2O3·13 H2O
(4CaO·Al2O3·Fe2O3) + 7 H2O → 3 CaO·Al2O3·6H2O + CaO·Fe2O3·H2O
And during the hardening (the chemistry of the reaction of hydration is still not completely clear):
(3CaO·SiO2)2 + (x+3) H2O → 3 CaO2·SiO2·xH2O + 3 Ca(OH)2
(2CaO·SiO2)2 + (x+1) H2O → 3 CaO2·SiO2·xH2O + Ca(OH)2
The silicates are responsible of the mechanical properties of the cement, the celite and the browmillerite are essential to allow
the formation of the liquid phase during the cooking.
History of the origin of cement
An early version of cement made with lime, sand, and gravel was used in Mesopotamia in the third millennium B.C. and later in
Egypt. It is uncertain where it was first discovered that a combination of hydrated non-hydraulic lime and a pozzolan produces a
hydraulic mixture (see also: Pozzolanic reaction), but concrete made from such mixtures was first used by the Ancient
Macedonians and three centuries later on a large scale by Roman engineers. They used both natural pozzolans (trass or
pumice) and artificial pozzolans (ground brick or pottery) in these concretes. Many excellent examples of structures made from
these concretes are still standing, notably the huge dome of the Pantheon in Rome and the massive Baths of Caracalla. The
vast system of Roman aqueducts also made extensive use of hydraulic cement.
Although any preservation of this knowledge in literary sources from the Middle Ages is unknown, medieval masons and some
military engineers maintained an active tradition of using hydraulic cement in structures such as canals, fortresses, harbors, and
shipbuilding facilities. The technical knowledge of making hydraulic cement was later formalized by French and British
engineers in the 18th century.
Modern hydraulic cements began to be developed from the start of the Industrial Revolution (around 1800), driven by three
Hydraulic cement render (stucco) for finishing brick buildings in wet climates.
Hydraulic mortars for masonry construction of harbor works, etc., in contact with sea water.
Development of strong concretes.
In Britain particularly, good quality building stone became ever more expensive during a period of rapid growth, and it became
a common practice to construct prestige buildings from the new industrial bricks, and to finish them with a stucco to imitate
stone. Hydraulic limes were favored for this, but the need for a fast set time encouraged the development of new cements. Most
famous was Parker's "Roman cement". This was developed by James Parker in the 1780s, and finally patented in 1796. It
was, in fact, nothing like any material used by the Romans, but was a "Natural cement" made by burning septaria – nodules that
are found in certain clay deposits, and that contain both clay minerals and calcium carbonate. The burnt nodules were ground to
a fine powder. This product, made into a mortar with sand, set in 5–15 minutes. The success of "Roman Cement" led other
manufacturers to develop rival products by burning artificial mixtures of clay and chalk.
John Smeaton made an important contribution to the development of cements when he was planning the construction of the
third Eddystone Lighthouse (1755–9) in the English Channel. He needed a hydraulic mortar that would set and develop some
strength in the twelve hour period between successive high tides. He performed an exhaustive market research on the available
hydraulic limes, visiting their production sites, and noted that the "hydraulicity" of the lime was directly related to the clay content
of the limestone from which it was made. Smeaton was a civil engineer by profession, and took the idea no further. Apparently
unaware of Smeaton's work, the same principle was identified by Louis Vicat in the first decade of the nineteenth century. Vicat
went on to devise a method of combining chalk and clay into an intimate mixture, and, burning this, produced an "artificial
cement" in 1817. James Frost, working in Britain, produced what he called "British cement" in a similar manner around
the same time, but did not obtain a patent until 1822. In 1824, Joseph Aspdin patented a similar material, which he called
Portland cement, because the render made from it was in color similar to the prestigious Portland stone.
Setting time and "early strength" are important characteristics of cements. Hydraulic limes, "natural" cements, and "artificial"
cements all rely upon their belite content for strength development. Belite develops strength slowly. Because they were burned
at temperatures below 1250 °C, they contained no alite, which is responsible for early strength in modern cements. The first
cement to consistently contain alite was made by Joseph Aspdin's son William in the early 1840s. This was what we call today
"modern" Portland cement. Because of the air of mystery with which William Aspdin surrounded his product, others (e.g., Vicat
and I.C. Johnson) have claimed precedence in this invention, but recent analysis of both his concrete and raw cement have
shown that William Aspdin's product made at Northfleet, Kent was a true alite-based cement. However, Aspdin's methods
were "rule-of-thumb": Vicat is responsible for establishing the chemical basis of these cements, and Johnson established the
importance of sintering the mix in the kiln.
William Aspdin's innovation was counterintuitive for manufacturers of "artificial cements", because they required more lime in the
mix (a problem for his father), a much higher kiln temperature (and therefore more fuel), and the resulting clinker was very hard
and rapidly wore down the millstones, which were the only available grinding technology of the time. Manufacturing costs were
therefore considerably higher, but the product set reasonably slowly and developed strength quickly, thus opening up a market
for use in concrete. The use of concrete in construction grew rapidly from 1850 onward, and was soon the dominant use for
cements. Thus Portland cement began its predominant role.
In the US the first large scale use of cement was Rosendale cement a natural cement mined from a massive deposit of a large
dolostone rock deposit discovered in the early 19th century near Rosendale, New York. Rosendale cement was extremely
popular for the foundation of buildings (e.g., Statue of Liberty, Capitol Building, Brooklyn Bridge) and lining water pipes. But
its long curing time of at least a month made it unpopular after World War One in the construction of highways and bridges and
many states and construction firms turned to the use of Portland cement. Because of the switch to Portland cement, by the end
of the 1920s of the 15 Rosendale cement companies, only one had survived. But in the early 1930s it was soon discovered
that, while Portland cement had a faster setting time it was not as durable, especially for highways, to the point that some states
stopped building highways and roads with cement. Bertrain H. Wait, an engineer whose company had worked on the
construction of the New York Cities Catskill Aqueduct, was impressed with the durability of Rosendale cement, and came up
with a blend of both Rosendale and synthetic cements which had the good attributes of both: it was highly durable and had a
much faster setting time. Mr. Wait convinced the New York Commissioner of Highways to construct an experimental section of
highway near New Paltz, New York, using one sack of Rosendale to six sacks of synthetic cement, and it was proved a
success and for decades the Rosendale-synthetic cement blend became common use in highway and bridge construction.
Types of modern cement
Main article: Portland cement
Cement is made by heating limestone (calcium carbonate) with small quantities of other materials (such as clay) to 1450 °C in a
kiln, in a process known as calcination, whereby a molecule of carbon dioxide is liberated from the calcium carbonate to form
calcium oxide, or quicklime, which is then blended with the other materials that have been included in the mix. The resulting hard
substance, called 'clinker', is then ground with a small amount of gypsum into a powder to make 'Ordinary Portland Cement',
the most commonly used type of cement (often referred to as OPC). Portland cement is a basic ingredient of concrete, mortar
and most non-specialty grout. The most common use for Portland cement is in the production of concrete. Concrete is a
composite material consisting of aggregate (gravel and sand), cement, and water. As a construction material, concrete can be
cast in almost any shape desired, and once hardened, can become a structural (load bearing) element. Portland cement may be
grey or white.
Energetically modified cement
Main article: Energetically modified cement
The grinding process to produce Energetically modified cement (EMC) yields materials made from pozzolanic minerals that
have been treated using a patented milling process ("EMC Activation"). This yields a high-level replacement of Portland
cement in concrete with lower costs, performance and durability improvements, with significant energy and carbon dioxide
savings. The resultant concretes can have the same, if not improved, physical characteristics as "normal" concretes, at a
fraction of the cost of using Portland cement.
Portland cement blends
Portland cement blends are often available as inter-ground mixtures from cement producers, but similar formulations are often
also mixed from the ground components at the concrete mixing plant. Portland blastfurnace cement contains up to 70%
ground granulated blast furnace slag, with the rest Portland clinker and a little gypsum. All compositions produce high ultimate
strength, but as slag content is increased, early strength is reduced, while sulfate resistance increases and heat evolution
diminishes. Used as an economic alternative to Portland sulfate-resisting and low-heat cements. Portland flyash cement
contains up to 35% fly ash. The fly ash is pozzolanic, so that ultimate strength is maintained. Because fly ash addition allows a
lower concrete water content, early strength can also be maintained. Where good quality cheap fly ash is available, this can be
an economic alternative to ordinary Portland cement. Portland pozzolan cement includes fly ash cement, since fly ash is a
pozzolan, but also includes cements made from other natural or artificial pozzolans. In countries where volcanic ashes are
available (e.g. Italy, Chile, Mexico, the Philippines) these cements are often the most common form in use. Portland silica
fume cement. Addition of silica fume can yield exceptionally high strengths, and cements containing 5–20% silica fume are
occasionally produced. However, silica fume is more usually added to Portland cement at the concrete mixer. Masonry
cements are used for preparing bricklaying mortars and stuccos, and must not be used in concrete. They are usually complex
proprietary formulations containing Portland clinker and a number of other ingredients that may include limestone, hydrated
lime, air entrainers, retarders, waterproofers and coloring agents. They are formulated to yield workable mortars that allow
rapid and consistent masonry work. Subtle variations of Masonry cement in the US are Plastic Cements and Stucco Cements.
These are designed to produce controlled bond with masonry blocks. Expansive cements contain, in addition to Portland
clinker, expansive clinkers (usually sulfoaluminate clinkers), and are designed to offset the effects of drying shrinkage that is
normally encountered with hydraulic cements. This allows large floor slabs (up to 60 m square) to be prepared without
contraction joints. White blended cements may be made using white clinker and white supplementary materials such as high-
purity metakaolin. Colored cements are used for decorative purposes. In some standards, the addition of pigments to produce
"colored Portland cement" is allowed. In other standards (e.g. ASTM), pigments are not allowed constituents of Portland
cement, and colored cements are sold as "blended hydraulic cements". Very finely ground cements are made from mixtures
of cement with sand or with slag or other pozzolan type minerals that are extremely finely ground together. Such cements can
have the same physical characteristics as normal cement but with 50% less cement particularly due to their increased surface
area for the chemical reaction. Even with intensive grinding they can use up to 50% less energy to fabricate than ordinary
Non-Portland hydraulic cements
Pozzolan-lime cements. Mixtures of ground pozzolan and lime are the cements used by the Romans, and can be found in
Roman structures still standing (e.g. the Pantheon in Rome). They develop strength slowly, but their ultimate strength can be
very high. The hydration products that produce strength are essentially the same as those produced by Portland cement. Slag-
lime cements. Ground granulated blast furnace slag is not hydraulic on its own, but is "activated" by addition of alkalis, most
economically using lime. They are similar to pozzolan lime cements in their properties. Only granulated slag (i.e. water-
quenched, glassy slag) is effective as a cement component. Supersulfated cements. These contain about 80% ground
granulated blast furnace slag, 15% gypsum or anhydrite and a little Portland clinker or lime as an activator. They produce
strength by formation of ettringite, with strength growth similar to a slow Portland cement. They exhibit good resistance to
aggressive agents, including sulfate. Calcium aluminate cements are hydraulic cements made primarily from limestone and
bauxite. The active ingredients are monocalcium aluminate CaAl2O4 (CaO · Al2O3 or CA in Cement chemist notation, CCN)
and mayenite Ca12Al14O33 (12 CaO · 7 Al2O3, or C12A7 in CCN). Strength forms by hydration to calcium aluminate
hydrates. They are well-adapted for use in refractory (high-temperature resistant) concretes, e.g. for furnace linings. Calcium
sulfoaluminate cements are made from clinkers that include ye'elimite (Ca4(AlO2)6SO4 or C4A3S in Cement chemist's
notation) as a primary phase. They are used in expansive cements, in ultra-high early strength cements, and in "low-energy"
cements. Hydration produces ettringite, and specialized physical properties (such as expansion or rapid reaction) are obtained
by adjustment of the availability of calcium and sulfate ions. Their use as a low-energy alternative to Portland cement has been
pioneered in China, where several million tonnes per year are produced. Energy requirements are lower because of the
lower kiln temperatures required for reaction, and the lower amount of limestone (which must be endothermically
decarbonated) in the mix. In addition, the lower limestone content and lower fuel consumption leads to a CO2 emission around
half that associated with Portland clinker. However, SO2 emissions are usually significantly higher. "Natural" cements
Global Cement Production in 2010
correspond to certain cements of the pre-Portland era, produced by burning argillaceous limestones at moderate temperatures.
The level of clay components in the limestone (around 30–35%) is such that large amounts of belite (the low-early strength,
high-late strength mineral in Portland cement) are formed without the formation of excessive amounts of free lime. As with any
natural material, such cements have highly variable properties. Geopolymer cements are made from mixtures of water-soluble
alkali metal silicates and aluminosilicate mineral powders such as fly ash and metakaolin.
Cement sets or cures when mixed with water which causes a series of hydration chemical reactions. The constituents slowly
hydrate and crystallize; the interlocking of the crystals gives cement its strength. Maintaining a high moisture content in cement
during curing increases both the speed of curing, and its final strength. Gypsum is often added to Portland cement to prevent
early hardening or "flash setting", allowing a longer working time. The time it takes for cement to cure varies depending on the
mixture and environmental conditions; initial hardening can occur in as little as twenty minutes, while full cure can take over a
month. Cement typically cures to the extent that it can be put into service within 24 hours to a week.
Bags of cement routinely have health and safety warnings printed on them because not only is cement highly alkaline, but the
setting process is exothermic. As a result, wet cement is strongly caustic and can easily cause severe skin burns if not promptly
washed off with water. Similarly, dry cement powder in contact with mucous membranes can cause severe eye or respiratory
irritation. Reducing agents are sometimes added to cement to prevent the formation of carcinogenic chromate in cement.
Cement users should wear protective clothing.
Cement industry in the world
See also: List of countries by cement
In 2010, the world production of hydraulic cement was
3,300 million tonnes. The top three producers were
China with 1,800, India with 220, and USA with 63.5
million tonnes for a combined total of over half the
world total by the world's three most populated
For the world capacity to produce cement in 2010, the
situation was similar with the top three states (China,
India, and USA) accounting for just under half the
world total capacity.
"For the past 18 years, China consistently has
produced more cement than any other country in the
world. [...] (However,) China's cement export peaked
in 1994 with 11 million tonnes shipped out and has
been in steady decline ever since. Only 5.18 million tonnes were exported out of China in 2002. Offered at $34 a ton, Chinese
cement is pricing itself out of the market as Thailand is asking as little as $20 for the same quality."
Global Cement Capacity in 2010
In 2006, it was estimated that China manufactured 1.235 billion tonnes of cement, which was 44% of the world total cement
production. "Demand for cement in China is expected to advance 5.4% annually and exceed 1 billion tonnes in 2008, driven
by slowing but healthy growth in construction expenditures. Cement consumed in China will amount to 44% of global demand,
and China will remain the world's largest national
consumer of cement by a large margin."
In 2010, 3.3 billion tonnes of cement was consumed
globally. Of this, China accounted for 1.8 billion
See also: Cement in Africa
Cement manufacture causes environmental impacts at
all stages of the process. These include emissions of
airborne pollution in the form of dust, gases, noise and
vibration when operating machinery and during blasting
in quarries, and damage to countryside from quarrying.
Equipment to reduce dust emissions during quarrying
and manufacture of cement is widely used, and
equipment to trap and separate exhaust gases are
coming into increased use. Environmental protection
also includes the re-integration of quarries into the countryside after they have been closed down by returning them to nature or
Carbon concentration in cement spans from ≈5% in cement structures to ≈8% in the case of roads in cement. Cement
manufacturing releases CO2 in the atmosphere both directly when calcium carbonate is heated, producing lime and carbon
dioxide, and also indirectly through the use of energy if its production involves the emission of CO2. The cement industry
produces about 5% of global man-made CO2 emissions, of which 50% is from the chemical process, and 40% from burning
fuel. The amount of CO2 emitted by the cement industry is nearly 900 kg of CO2 for every 1000 kg of cement produced.
 The high proportion of carbon dioxide produced in the chemical reaction leads to large decrease in mass in the conversion
from limestone to cement. So, to reduce the transport of heavier raw materials and to mimimize the associated costs, it is more
economical for cement plants to be closer to the limestone quarries rather than to the consumer centers.
In certain applications, lime mortar reabsorbs the same amount of CO2 as was released in its manufacture, and has a lower
energy requirement in production than mainstream cement. Newly developed cement types from Novacem and Eco-cement
can absorb carbon dioxide from ambient air during hardening. Use of the Kalina cycle during production can also increase
Heavy metal emissions in the air
In some circumstances, mainly depending on the origin and the composition of the raw materials used, the high-temperature
calcination process of limestone and clay minerals can release in the atmosphere gases and dust rich in volatile heavy metals,
a.o, thallium, cadmium and mercury are the most toxic. Heavy metals (Tl, Cd, Hg, ...) are often found as trace elements in
common metal sulfides (pyrite (FeS2), zinc blende (ZnS), galena (PbS), ...) present as secondary minerals in most of the raw
materials. Environmental regulations exist in many countries to limit these emissions. As of 2011 in the United States, cement
kilns are "legally allowed to pump more toxins into the air than are hazardous-waste incinerators."
Heavy metals present in the clinker
The presence of heavy metals in the clinker arises both from the natural raw materials and from the use of recycled by-products
or alternative fuels. The high pH prevailing in the cement porewater (12.5 < pH < 13.5) limits the mobility of many heavy metals
by decreasing their solubility and increasing their sorption onto the cement mineral phases. Nickel, zinc and lead are commonly
found in cement in non-negligible concentrations.
Use of alternative fuels and by-products materials
A cement plant consumes 3 to 6 GJ of fuel per tonne of clinker produced, depending on the raw materials and the process
used. Most cement kilns today use coal and petroleum coke as primary fuels, and to a lesser extent natural gas and fuel oil.
Selected waste and by-products with recoverable calorific value can be used as fuels in a cement kiln (referred to as co-
processing), replacing a portion of conventional fossil fuels, like coal, if they meet strict specifications. Selected waste and by-
products containing useful minerals such as calcium, silica, alumina, and iron can be used as raw materials in the kiln, replacing
raw materials such as clay, shale, and limestone. Because some materials have both useful mineral content and recoverable
calorific value, the distinction between alternative fuels and raw materials is not always clear. For example, sewage sludge has a
low but significant calorific value, and burns to give ash containing minerals useful in the clinker matrix.
Green cement is a cementitious material that meets or exceeds the functional performance capabilities of ordinary Portland
cement by incorporating and optimizing recycled materials, thereby reducing consumption of natural raw materials, water, and
energy, resulting in a more sustainable construction material.
The manufacturing process for green cement succeeds in reducing, and even eliminating, the production and release of
damaging pollutants and greenhouse gasses, particularly CO2.
Bangladesh Cement Manufacturers Association (BCMA)
Cement chemist notation
Energetically Modified Cement
1. ^ Gartner, Ellis; Macphee, Donald (2011). "A physico-chemical basis for novel cementitious binders". Cement and Concrete
Research 41 (7): 736–749. doi:10.1016/j.cemconres.2011.03.006 (http://dx.doi.org/10.1016%2Fj.cemconres.2011.03.006).
2. ^ Brabant, Malcolm (12 April 2011). Macedonians created cement three centuries before the Romans
3. ^ Heracles to Alexander The Great: Treasures From The Royal Capital of Macedon, A Hellenic Kingdom in the Age of
Democracy (http://www.ashmolean.org/exhibitions/current/?timing=current&id=57&exhibitionYear=2011), Ashmolean
Museum of Art and Archaeology, University of Oxford
4. ^ Hill, Donald (1984). A History of Engineering in Classical and Medieval Times, Routledge, p. 106, ISBN 0415152917.
5. ^ Pure natural pozzolan cement
6. ^ Russo, Ralph (2006) "Aqueduct Architecture: Moving Water to the Masses in Ancient Rome"
(http://www.yale.edu/ynhti/curriculum/units/2006/4/06.04.04.x.html), in Math in the Beauty and Realization of Architecture,
Vol. IV, Curriculum Units by Fellows of the Yale-New Haven Teachers Institute 1978–2012, Yale-New Haven Teachers
7. ^ a b Sismondo, Sergio (2009). An Introduction to Science and Technology Studies (http://books.google.com/books?
id=LescwF8FBigC). John Wiley and Sons, 2nd edition, p. 142. ISBN 978-1-4051-8765-7.
8. ^ Mukerji, Chandra (2009). Impossible engineering: technology and territoriality on the Canal du Midi
(http://books.google.com/books?id=fRwNRrFswv8C&dq). Princeton University Press, p. 121, ISBN 978-0-691-14032-2.
9. ^ Francis, A.J. (1977) The Cement Industry 1796–1914: A History, David & Charles, 1977, ISBN 0-7153-7386-2, Ch. 2.
10. ^ "Who Discovered Cement" (http://www.nationalcement.com/faq/who-discovered-cement).
11. ^ Francis, A.J. (1977) The Cement Industry 1796–1914: A History, David & Charles, 1977, ISBN 0-7153-7386-2, Ch. 5.
12. ^ Hewlett, Peter (2003). Lea's Chemistry of Cement and Concrete (http://books.google.com/books?id=v1JVu4iifnMC).
Butterworth-Heinemann. p. Ch. 1. ISBN 978-0-08-053541-8.
13. ^ "Natural Cement Comes Back" (http://books.google.com/books?id=VCcDAAAAMBAJ&pg=PA118), October 1941, Popular
14. ^ Performance of Energetically Modified Cement (EMC) and Energetically Modified Fly Ash (EMFA) as Pozzolan
15. ^ Ronin, V; Jonasson, J-E; Hedlund, H (1999). "Ecologically effective performance Portland cement-based binders",
proceedings in Sandefjord, Norway 20–24 June 1999. Norway: Norsk Betongforening. pp. 1144–1153.
16. ^ a b Justnes, Harald; Elfgren, Lennart; Ronin, Vladimir (2005). "Mechanism for performance of energetically modified cement
versus corresponding blended cement"
Cement and Concrete Research 35 (2): 315–323. doi:10.1016/j.cemconres.2004.05.022
17. ^ Kosmatka, S.H.; Panarese, W.C. (1988). Design and Control of Concrete Mixtures. Skokie, IL, USA: Portland Cement
Association. pp. 17, 42, 70, 184. ISBN 0-89312-087-1.
18. ^ U.S. Federal Highway Administration. "Ground Granulated Blast-Furnace Slag"
(http://www.fhwa.dot.gov/infrastructure/materialsgrp/ggbfs.htm). Retrieved 24 January 2007.
19. ^ U.S. Federal Highway Administration. "Fly Ash" (http://www.fhwa.dot.gov/infrastructure/materialsgrp/flyash.htm). Retrieved
24 January 2007.
20. ^ U.S. Federal Highway Administration. "Silica Fume" (http://www.fhwa.dot.gov/infrastructure/materialsgrp/silica.htm).
Retrieved 24 January 2007.
21. ^ Bye G.C. (1999), Portland Cement 2nd Ed., Thomas Telford, 1999, ISBN 0-7277-2766-4, pp. 206–208
22. ^ Zhang L., Su M., Wang Y., Development of the use of sulfo- and ferroaluminate cements in China in Adv. Cem. Res. 11 N
°1, pp. 15–21.
23. ^ CIS26 – cement (http://www.hse.gov.uk/pubns/cis26.pdf). (PDF) . Retrieved on 5 May 2011.
24. ^ "Mother left with horrific burns to her knees after kneeling in B&Q cement while doing kitchen DIY"
Daily Mail (London). 15 February 2011.
25. ^ Pyatt, Jamie (15 February 2011). "Mums horror cement burns"
(http://www.thesun.co.uk/sol/homepage/news/3412957/Mums-horror-cement-burns.html). The Sun (London).
26. ^ United States Geological Survey. "USGS Mineral Program Cement Report. (Jan 2011)"
27. ^ Edwards, P; McCaffrey, R. Global Cement Directory 2010. PRo Publications (http://www.globalcement.com). Epsom, UK,
28. ^ Yan, Li Yong (7 January 2004) China's way forward paved in cement
(http://www.atimes.com/atimes/China/FA07Ad02.html), Asia Times
29. ^ China now no. 1 in CO2 emissions; USA in second position: more info
(http://www.mnp.nl/en/dossiers/Climatechange/moreinfo/Chinanowno1inCO2emissionsUSAinsecondposition.html), NEAA (19
30. ^ China's cement demand to top 1 billion tonnes in 2008
CementAmericas (1 November 2004).
31. ^ Coal and Cement (http://www.worldcoal.org/coal/uses-of-coal/coal-cement/). worldcoal.org
32. ^ Scalenghe, R., Malucelli, F., Ungaro, F., Perazzone, L., Filippi, N., Edwards, A.C. (2011). "Influence of 150 years of land
use on anthropogenic and natural carbon stocks in Emilia-Romagna Region (Italy)". Environmental Science & Technology 45
(12): 5112–5117. doi:10.1021/es1039437 (http://dx.doi.org/10.1021%2Fes1039437).
33. ^ EIA – Emissions of Greenhouse Gases in the U.S. 2006-Carbon Dioxide Emissions
(http://www.eia.doe.gov/oiaf/1605/ggrpt/carbon.html). US Department of Energy.
34. ^ The Cement Sustainability Initiative: Progress report (http://www.wbcsd.org/includes/getTarget.asp?type=d&id=ODY3MA),
World Business Council for Sustainable Development (1 June 2002).
35. ^ Mahasenan, Natesan; Steve Smith, Kenneth Humphreys, Y. Kaya (2003). "The Cement Industry and Global Climate Change:
Current and Potential Future Cement Industry CO2 Emissions" (http://www.sciencedirect.com/science/article/B873D-
4P9MYFN-BK/2/c58323fdf4cbc244856fe80c96447f44). Greenhouse Gas Control Technologies – 6th International
Conference. Oxford: Pergamon. pp. 995–1000. ISBN 978-0-08-044276-1. Retrieved 9 April 2008.
36. ^ Chandak, Shobhit. "Report on cement industry in India" (http://www.scribd.com/doc/13378451/Cement-Industry-In-India).
scribd. Retrieved 21 July 2011.
37. ^ Novacem (http://www.imperialinnovations.co.uk/?q=node/176). imperialinnovations.co.uk
38. ^ Jha, Alok (31 December 2008). "Revealed: The cement that eats carbon dioxide"
(http://www.guardian.co.uk/environment/2008/dec/31/cement-carbon-emissions). The Guardian (London). Retrieved 28 April
39. ^ "Factsheet on: Thallium" (http://www.epa.gov/safewater/pdfs/factsheets/ioc/thallium.pdf). Retrieved 15 September 2009.
40. ^ Berkes, Howard (10 November 2011). "EPA Regulations Give Kilns Permission To Pollute : NPR"
(http://www.npr.org/2011/11/10/142183546/epa-regulations-give-kilns-permission-to-pollute). NPR.org. Retrieved 17
41. ^ Guidelines for the Selection and Use of Fuels and Raw Materials in the Cement Manufacturing Process
(http://www.wbcsd.org/DocRoot/Vjft3qGjo1v6HREH7jM6/tf2-guidelines.pdf), World Business Council for Sustainable
Development (1 June 2005).
Aitcin, Pierre-Claude (2000). "Cements of yesterday and today: Concrete of tomorrow". Cement and Concrete
Research 30 (9): 1349–1359. doi:10.1016/S0008-8846(00)00365-3 (http://dx.doi.org/10.1016%2FS0008-
van Oss, Hendrik G.; Padovani, Amy C. (2002). "Cement Manufacture and the Environment, Part I: Chemistry and
Technology". Journal of Industrial Ecology 6 (1): 89–105. doi:10.1162/108819802320971650
van Oss, Hendrik G.; Padovani, Amy C. (2003). "Cement Manufacture and the Environment, Part II: Environmental
Challenges and Opportunities". Journal of Industrial Ecology 7 (1): 93–126. doi:10.1162/108819803766729212
Friedrich W. Locher: Cement : Principles of production and use, Düsseldorf, Germany: Verlag Bau + Technik
GmbH, 2006, ISBN 3-7640-0420-7
Javed I. Bhatty, F. MacGregor Miller, Steven H. Kosmatka; editors: Innovations in Portland Cement
Manufacturing, SP400, Portland Cement Association, Skokie, Illinois, USA, 2004, ISBN 0-89312-234-3
"Cement Industry Is at Center of Climate Change Debate"
(http://www.nytimes.com/2007/10/26/business/worldbusiness/26cement.html) article by Elizabeth Rosenthal in the New
York Times 26 October 2007
Neville, A.M. (1996). Properties of concrete. Fourth and final edition standards. Pearson, Prentice Hall. ISBN 0-
582-23070-5. OCLC 33837400 (//www.worldcat.org/oclc/33837400).
Taylor, H.F.W. (1990). Cement Chemistry. Academic Press. p. 475. ISBN 0-12-683900-X.
Ulm, Franz-Josef; Roland J.-M. Pellenq, Akihiro Kushima, Rouzbeh Shahsavari, Krystyn J. Van Vliet, Markus J.
Buehler, Sidney Yip (2009). "A realistic molecular model of cement hydrates". Proceedings of the National Academy
of Sciences 106 (38): 16102–16107. doi:10.1073/pnas.0902180106
Energetically Modified Cement (http://www.emccement.com)
Cement's basic molecular structure finally decoded (MIT, 2009) (http://cee.mit.edu/cee-in-focus/2011/spring/cement-
British Cement Association (UK) (http://www.cementindustry.co.uk/)
Cembureau (EU) (http://www.cembureau.be/)
Portland Cement Association (US) (http://www.cement.org/)
Verein Deutscher Zementwerke e. V. (VDZ), (Germany) (http://www.vdz-online.de/home1.html?lang=en)
Carbon dioxide emission from the global cement industry (in 1994)
World Business Council for Sustainable Development: Cement Sustainability Initiative (http://www.wbcsdcement.org/)
How is Cement Made? Flash Animation (http://www.cemex.co.uk/ce/ce_pp.asp)
Cement Mixers (http://www.hi-unique.com/)
Cement by the Barrel and Cask (http://espace.library.uq.edu.au/view.php?pid=UQ:9029), Concrete in Australia, 26 3:
Chemistry of Concrete (http://www.periodicvideos.com/videos/mv_concrete.htm) at The Periodic Table of Videos
(University of Nottingham)
Retrieved from "http://en.wikipedia.org/w/index.php?title=Cement&oldid=565527050"
Categories: Cement Concrete Building materials
This page was last modified on 23 July 2013 at 20:35.
Text is available under the Creative Commons Attribution-ShareAlike License; additional terms may apply. By using this
Wikipedia® is a registered trademark of the Wikimedia Foundation, Inc., a non-profit organization.